Preparation and nanoencapsulation of l-asparaginase II in chitosan-tripolyphosphate nanoparticles and in vitro release study
© Bahreini et al.; licensee Springer. 2014
Received: 15 March 2014
Accepted: 9 June 2014
Published: 9 July 2014
This paper describes the production, purification, and immobilization of l-asparaginase II (ASNase II) in chitosan nanoparticles (CSNPs). ASNase II is an effective antineoplastic agent, used in the acute lymphoblastic leukemia chemotherapy. Cloned ASNase II gene (ansB) in pAED4 plasmid was transformed into Escherichia coli BL21pLysS (DE3) competent cells and expressed under optimal conditions. The lyophilized enzyme was loaded into CSNPs by ionotropic gelation method. In order to get optimal entrapment efficiency, CSNP preparation, chitosan/tripolyphosphate (CS/TPP) ratio, and protein loading were investigated. ASNase II loading into CSNPs was confirmed by Fourier transform infrared (FTIR) spectroscopy, and morphological observation was carried out by transmission electron microscopy. Three absolute CS/TPP ratios were studied. Entrapment efficiency and loading capacity increased with increasing CS and TPP concentration. The best ratio was applied for obtaining optimal ASNase II-loaded CSNPs with the highest entrapment efficiency. Size, zeta potential, entrapment efficiency, and loading capacity of the optimal ASNase II-CSNPs were 340 ± 12 nm, 21.2 ± 3 mV, 76.2% and 47.6%, respectively. The immobilized enzyme showed an increased in vitro half-life in comparison with the free enzyme. The pH and thermostability of the immobilized enzyme was comparable with the free enzyme. This study leads to a better understanding of how to prepare CSNPs, how to achieve high encapsulation efficiency for a high molecular weight protein, and how to prolong the release of protein from CSNPs. A conceptual understanding of biological responses to ASNase II-loaded CSNPs is needed for the development of novel methods of drug delivery.
KeywordsEnzyme immobilization Optimization Ionotropic gelation Nanoparticle Cross-linking Half-life
l-Asparaginase II (ASNase II) is an enzyme that is widely used for the treatment of hematopoietic diseases such as acute lymphoblastic leukemia. The enzyme is able to destroy asparagine-dependent tumors by degrading circulating l-asparagine and destroying malignant cells [1, 2]. However, native ASNase II is associated with a high incidence of allergic reactions. Due to the formation of neutralizing antibodies, the half-life of circulating ASNase II (18 to 24 h) can be shortened to approximately 2.5 h . Moreover, it is susceptible to proteolytic degradation by the proteases of the host organism. Much effort has been devoted to develop methods to avoid such side effects as well as to increase its in vivo half-life. For example, ASNase II has been chemically modified by polyethyleneglycol , poly-(d,l-alanine) , and dextran .
In the recent years, nanotechnology has shown a significant promise in the preparation of immobilized enzymes. Immobilization of enzymes onto biopolymer nanoparticles may result in some benefits, such as improving their stability to pH and temperature, as well as resistance to proteases and other denaturing compounds. Candidate carrier biopolymers should exhibit chemical and physical stability, biological compatibility, high purity, homogeneous molecular weight (MW) distribution, and adequate functional groups for binding to biomolecules with high loading capacity. They exhibit several drug loading mechanisms including electrostatic attractions, hydrophobic interactions, and covalent binding. They can form a matrix or membrane that can slow drug release over a prolonged period, avoiding repetitive dosing. However, one should bear in mind that covalent coupling of enzymes to polymers may result in conformational alterations, pharmacokinetic modifications, and a significant decrease in enzymatic activity. Examples of such biopolymer nanoparticles that ASNase II has already been incorporated in are liposomes , poly(d,l-lactide-co-glycolide) (PLGA) , and hydrogel-magnetic nanoparticles .
Chitosan (CS), produced by alkaline N-deacetylation of chitin, is another natural polymer that has good physicochemical (reactive OH and NH2 groups), as well as biological properties. It is composed of glucosamine and N-acetylglucosamine monomers linked by β [1–4] glycosidic bonds. CS is hydrophilic and soluble in acidic solutions by protonation of the amine groups. It is degraded by enzymes such as lysozymes, some lipases, and proteases. CS is a biologically safe, non-toxic, biocompatible, and biodegradable polysaccharide . Current research with CS focuses on its use as a novel drug, gene, peptide, and vaccine delivery vehicle and as a scaffold for targeted drug delivery and tissue engineering applications [11, 12].
Two groups of cross-linkers are usually employed to obtain CS particles. One group, such as glutaraldehyde and glucomannan, cross-links through covalent bonds leading to quite stable matrixes. The other group is ionic cross-linkers that cross-link through ionic gelation and electrostatic interactions between the positively charged chitosan chains and polyanions. The polyanion most commonly used for the ionic cross-linking is tripolyphosphate (TPP), which is non-toxic. Due to the proved toxicity of glutaraldehyde and other organic molecules used in the synthesis of gels covalently stabilized, only the second synthesis technique (ionic gelation) can be used for pharmaceutical applications.
Bodmeier et al.  and Calvo et al.  used an ionotropic gelation method to prepare CS particles with sizes ranging from micron to submicron for the first time, and this is a currently widely used method for preparing CSNPs. In this method, an anionic cross-linking agent is introduced into an aqueous solution of CS in acetic acid. The cross-linking structure of the CS/TPP system is mainly determined by the reaction between the amino groups of CS and TPP ions, and this reaction depends strongly on the associated pH [15, 16]. Alteration in the parameters such as cross-linker concentration, drug/polymer ratio, and processing conditions affects the morphology of CSNPs and the release rate of the loaded drug [17, 18].
Formulation development and optimization is a very critical process in the design and manufacture of any therapeutic drug. Depending on the design and delivery aims for a particular drug, the process requires several in vitro and in vivo study stages. Generally, the in vitro property is the rate or extent of drug dissolution and its release, whereas the in vivo study involves the plasma drug concentration, absorption, body interactions, and any possible side effects. The purpose of the in vitro study in the early stage of nanodrug development is to investigate the optimum formulation, evaluate the active ingredient, and assess any minor changes for drug development. The aim of the present work was to assess the in vitro preparation of ASNase II-loaded CSNPs cross-linked with TPP and to evaluate their efficacy for the entrapment and controlled release of the protein. The values were expressed as the averages of at least three independent experiments each.
The following materials were used: BL21 pLysS (DE3) strain (Novagen, Cat. No.: 69451–3, Darmstadt, Germany), pAED4 (BV Tech, Sofia, Bulgaria), isopropyl β-d-1-thiogalactopyranoside or IPTG (Sigma-Aldrich Cat. No.: I6758, St. Louis, MO, USA), Luria Bertani broth or LB broth (Merck, Cat. No.: 1.10285.0500, Whitehouse Station, NJ, USA), diethylaminoethyl (DEAE)-Sepharose Fast Flow (Amersham, Cat. No.: 17-0709-01, Amersham, UK), Sephadex G-75 (Sigma-Aldrich, Cat. No.: G7550), l-asparagine (Sigma-Aldrich, Cat. No.: A0884), Nessler's reagent (Sigma-Aldrich, Cat. No.: 72190), and CS (low molecular weight (% deacetylation 75% to 85%, viscosity 20 to 300 cP, average MW ~ 50 kDa), Sigma-Aldrich; Cat. No.: 448869), sodium tripolyphosphate (Sigma-Aldrich, Cat. No.: 238503).
ASNase II production, extraction, and purification
According to our optimized protocol for overproduction of recombinant protein , ASNase II (EC 188.8.131.52) was expressed in transformed Escherichia coli BL21 pLysS (DE3). The periplasmic ASNase II was extracted from the bacterial pellet using modified alkaline lysis method . The extract was clarified by centrifugation for 30 min at 30,000 × g at 4°C, and the supernatant was filtered through a 0.45-μm sterile filter. A single-step purification of ASNase II was performed by loading the filtrate sample onto the DEAE-Sepharose Fast Flow column (5 cm × 15 cm) pre-equilibrated with phosphate buffer (0.01 mM, pH 7.0). After removing the unbound proteins from the column by passing phosphate buffer, NaCl gradient from 50 to 200 mM was applied to the column at a flow rate of 4 ml/min. The collected fractions were analyzed for enzyme activity (U/ml) and protein content (mg/ml). The purity of ASNase II was judged using sodium dodecyl sulfate-polyacrylamide gel electrophoresis (SDS-PAGE) (15%) stained with Coomassie brilliant blue. The fractions with the higher ASNase II activity were pooled and analyzed for total activity (U), total protein level (mg), and specific activity (U/mg).
The purified solution from the previous step was desalted using Sephadex G-75 column (3.0 × 70 cm) pre-equilibrated with double-distilled water (DDW) at a flow rate of 3 ml/min. The most active fractions were pooled and concentrated by lyophilization (−50°C) and the protein powder was stored at 4°C.
Estimation of ASNase II activity
The activity of ASNase II was assayed using the Nessler method . A reaction mixture contained 0.5 ml Tris–HCl buffer (0.1 M, pH 8.5), 0.25 ml l-asparagine (10 mM in Tris–HCl buffer), and 25 μl of the enzymatic solution. After 15 min of incubation at 37°C, the reaction was terminated by the addition of 0.25 ml of 15% trichloroacetic acid (TCA). The liberated ammonia was determined by adding 0.25 ml of Nessler's reagent. The absorbance was recorded at 425 nm after 10 min. The absorbance values were converted to micromoles of ammonia using a standard curve prepared with ammonium sulfate. One unit of enzyme activity (IU) was defined as the amount of enzyme required to release 1 μmol of ammonia per minute under standard assay conditions.
Estimation of protein concentration
Protein concentration was estimated with Folin phenol reagent (Lowry method) using bovine serum albumin as a standard .
Preparation of CSNPs
CSNPs were prepared based on the ionotropic gelation method  with a small modification. The method is based on electrostatic interactions between the amine group of CS and the negatively charged group of TPP as a polyanion. During the process involving chemical reaction, CS undergoes ionotropic gelation and precipitates to form spherical particles that are distinguishable by opalescence of solution.
Low molecular weight CS was dissolved in DDW containing 1.2% acetic acid to a concentration of 0.5% (w/v) as stock solution. The isoelectric point of ASNase II and pKα of CS are 4.9  and 6.5 [24, 25], respectively. The pH of the CS solution was adjusted to 5.7 by NaOH as the mean pH point. TPP with the concentration of 0.5% (w/v) in DDW was prepared as the stock solution. Both solutions were filtered through a 0.25-μm sterile filter.
Preparation of ASNase II-CSNPs
ASNase II activity against CS and TPP
In order to determine the individual effect of each CS and TPP on ASNase II activity, 1 ml CS solution (0.2% (w/v), pH ~ 5.7) and 1 ml TPP solution (0.1% (w/v), pH ~ 8.5) were prepared from stocks. One milligram of lyophilized ASNase II was added to each solution, and both of them were slowly shaken for 15 min. The percentage of the preserved activity for both solutions was calculated based on the activity of untreated ASNase II (1 mg/ml), which was taken as 100%.
Two ways of preparation of the ASNase II-loaded CSNPs
The preparation of the ASNase II-loaded CSNPs via the ionotropic gelation method was examined in two ways. In the first approach, 1 mg of lyophilized protein was mixed with 1 ml of TPP solution (0.1% (w/v)), and the mixture was added dropwise to 1 ml of CS solution (0.2% (w/v)) with stirring using a magnetic stirrer. In the second method, 1 mg of lyophilized protein was mixed with 1 ml of CS solution (0.2% (w/v)), and TPP (0.1% (w/v)) was added dropwise to the protein/CS mixture with stirring. After 10 min of stirring, each opalescent solution was centrifuged (25,000 × g, 25°C for 30 min), and the amounts of the free protein in each supernatant were measured in order to analyze the entrapment efficiency.
Optimization of CS and TPP concentrations
Chitosan concentrations, TPP volumes from TPP stock solution (0.5% w / v ), and final TPP concentrations in final prepared nanoparticle suspensions
CS (% w/ v)
TPP (% w/ v)
Optimization of protein loading
The stable and suitable CS/TPP ratio from the previous step was selected in order to investigate the optimal entrapment efficiency and loading capacity of CSNPs, loaded with five different amounts of protein (1, 2, 3, 4, and 5 mg). Nanoparticles were prepared according to the procedure given above by adding a certain amount of lyophilized ASNase II in 1 ml of optimal CS solution. After centrifugation, the supernatants were separated to estimate the entrapment efficiency. The pellets of the particles in glycerol were suspended in 1 ml of DDW and dispersed by sonication. The size (nm), zeta potential (mV), protein content (mg), entrapment efficiency (%), and loading capacity (%) of the particles were determined.
Entrapment efficiency estimation
Loading capacity estimation
Characterization of ASNase II-loaded CSNPs
Particle size and zeta potential of ASNase II-CSNPs
The particle size, size distribution (polydispersity index (PDI)), and zeta potential of particles were measured by Zetasizer (Malvern Instruments, Worcestershire, UK), based on the dynamic light scattering (DLS) technique. The mean particle size was approximated as the z-average diameter and the width of the distribution as the PDI. DLS measurements were performed at 25°C with a detection angle of 90°. All measurements were preformed in triplicate, and the results were reported as mean ± standard deviation.
Fourier transform infrared spectroscopy
Fourier transform infrared (FTIR) spectroscopy (Bruker, Ettlingen, Germany) was used to characterize bonding characteristics of the lyophilized ASNase II, CS, CSNPs, and ASNase II-CSNPs.
Examinations of surface morphology and size distribution for CSNPs and ASNase II-loaded CSNPs were performed using a transmission electron microscope (TEM) (Philips CM30, Eindhoven, The Netherlands). About 5 μl of the nanoparticle solution was placed on a copper grid and stained with 2% (w/v) phosphotungstic acid.
In vitro ASNase II release
ASNase II release from the matrix complex was evaluated in three solutions of glycerol (5%)-phosphate-buffered saline (PBS) solution (pH 7.4), PBS solution (pH 7.4), and DDW containing 5% glycerol (pH 7.0). ASNase II-loaded CSNPs with the highest protein loading capacity were suspended in each of these solutions and incubated at 37°C. At predetermining time points, nanoparticles were collected with a centrifuge (25,000 × g, 30 min and 25°C). The supernatant was removed for protein content assay.
where %L represents the percentage of leakage, M o is the mass of ASNase II in the supernatant, and M e is the mass of entrapped ASNase II.
Effect of pH on enzyme activity and stability
The activities of the immobilized and free ASNase II were evaluated at different pH values in the range between pH 6.5 and 10 adjusted with Tris–HCl (0.1 M). In the case of pH stability experiment, the immobilized and free enzymes were incubated for 24 h at 4°C ± 1°C at different pH values (pH 6 to 10) in the absence of the substrate, and the residual activity was determined. The percentage of residual activities was calculated based on the untreated control activity, which was taken as 100%.
Effect of temperature on enzyme stability
Thermostability studies were carried out by pre-incubating the immobilized and free ASNase II at different temperatures (37°C, 45°C, 50°C, 60°C, 70°C, 80°C, and 90°C) for 60 min, followed by cooling. The percentage of residual activities was determined and calculated based on the untreated control activity, which was taken as 100%.
Half-life determination of the free and immobilized ASNase II
The solutions of Tris–HCl (0.1 M, pH = 8.5), DDW-glycerol (5%), and PBS-glycerol (5%) were considered for measuring the half-life of the free and immobilized enzyme. Solutions of the immobilized and free enzyme were slowly homogenized and incubated at 37°C to measure the half-life of both. At the time interval of 1, 3, 6, and 24 h, a sampling was done without replacement for the determination of enzymatic activity.
Results and discussion
Production and purification of ASNase II
Purification table of ASNase II by DEAE-Sepharose
Total protein (mg)
Total activity (U)
Specific activity (U/mg)
Before purification (filtrate)
After purification (DEAE-Sepharose)
Chloride (which would interfere with TPP in preparation of ionotropic nanoparticles) was eliminated from the DEAE-chromatographic product by Sephadex G-75 and the protein was lyophilized. At the high ionic strengths, the CS-TPP binding would be weakened to the point that the nanoparticles would cease to form , due to the competitive reaction between Cl− and TPP ions for NH3+.
Preparation of ASNase II-loaded CSNPs
ASNase II activity in CS and TPP solutions
Both CS and TPP have their characteristic charge and may likely affect ASNase II stability and activity. The behavior of ASNase II in the CS and TPP solutions was individually investigated before preparation of nanoparticles. The percentages of the preserved ASNase II activity in CS and TPP were 85% and 80% of the activity of untreated enzyme, respectively. This result can be explained from the standpoint of pH. As will be mentioned below, the optimum pH for the activity of free ASNase II is between 8.5 and 9 and enzyme activity decreases to about 86% at pH ~ 6.5. Most of the decrease in ASNase II activity in the case of CS could be attributed to the low pH of the CS solution (pH = 5.7). TPP was dissolved in DDW, and pH of the resulted solution was about 8.5 which is close to the optimum pH of free ASNase II activity. Thus, the decrease in ASNase II activity may be attributed to the effect of TPP on ASNase II, such as repulsion between the negative charges on TPP and ASNase II, the latter being negatively charged at pH 8.5.
Two ways for ASNase II-CSNP preparation
We compared the two methods of preparation of ASNase II-loaded CSNPs through ionotropic gelation method. The entrapment efficiency, size, and zeta potential of the nanoparticles prepared through adding ASNase II-TPP into CS solution were 61%, 143 ± 5 nm, and +35.4 ± 2 mV, whereas they were 68%, 140 ± 4 nm, and +34.9 ± 2 mV when TPP was added into ASNase II-CS solution. No significant differences were seen in the size and zeta potential between the two groups of nanoparticles, but the entrapment efficiency of the nanoparticles which resulted from adding TPP into ASNase II-CS solution was significantly higher than when ASNase II-TPP was added into the CS solution. This observation can be explained by possible interactions of ASNase II molecules with CS polymer before the addition of the cross-linker.
Since proteins are large macromolecules with flexible structure and are able to fold and unfold at different conditions, their interactions with long cationic CS chain and the resulting encapsulation can be complicated, depending on 3-D conformation, electrostatics, and the condition of solution. The polycationic CS chain has a flexible helical conformation in the relatively acidic solution (pH ~ 5.7), due to electrostatic repulsion forces which exist among the protonated amine groups, either within or between polymer chains. The CS chains possess three functional groups for chemical interaction: two hydroxyl groups (primary or secondary) and one primary amine. The negatively charged carboxyl groups on the surface of ASNase II could form electrostatic interactions with the positively charged amine groups and make hydrogen bonds with the hydroxyl groups of the CS chains. Such attachments of a spherical protein molecule did not completely suppress the positive surface charge of CS molecules. Therefore, a high proportion of amine groups on the CS chain might remain free and ready to form cross-links with TPP .
As CS is a highly charged polymer at pH ~ 5.7 (below its pKα ~ 6.5), it tends to form ion pairs with TPP as a polyvalent anion. At acidic pH, ionotropic cross-linking is the only way of neutralization of protonated CS by TPP ions. Dissolved sodium tripolyphosphate in water dissociates to give both hydroxyl and TPP ions (pH ~ 8.5). OH− and TPP ions in the acidic CS solution could compete to interact with the -NH3+ of CS, but OH− ions would be immediately neutralized by H+ ions and increase the pH of the CS solution. Therefore, by adding TPP, a competition would occur between ionotropic cross-linking by a polyanion and neutralization through deprotonation of CS. Ionotropic cross-linking is an important property which is broadly used in ionotropic gelation processes.
The mild effect of CS on the activity of ASNase II and the higher entrapment efficiency indicated adding TPP into the protein-CS solution as the selected way for nanoparticle preparation in the next steps.
Optimization of CS and TPP concentrations
CSNPs were prepared by certain amounts of CS (containing 1 mg ASNase II) and TPP. Increasing TPP volume or decrease in CS/TPP ratio led to increased turbidity, indicating a shift in the size variation of the particles to larger dimensions. Optimization of the CS/TPP ratio revealed that when this ratio declined to 0.2/0.06, 0.3/0.08, and 0.4/0.11, high turbidity appeared from the increased aggregation of the nanoparticles. Thus, the CS/TPP ratios of 0.2/0.06, 0.3/0.08, and 0.4/0.11 (Table 1) were discarded because of aggregation which was confirmed microscopically [14, 30].
Nanoparticle aggregation occurs under circumstances such as the rise in pH of suspension , inadequate speed of homogenization, or high level of cross-linker . López et al.  suggested that since the pKα value of the chitosan is close to the neutral pH, particles spontaneously aggregate in slightly basic pH, where they become completely uncharged. The final pH of the prepared ASNase II-loaded CSNP suspensions was between 6.2 and 6.3 in all CS/TPP ratios, which was lower than the pKα of chitosan. Moreover, increase in TPP concentration might be a more important agent for particle aggregation via cross-linking, as was observed through a raise in TPP volume. Aggregation might be prevented by using a high-speed homogenizer or by sonication during CSNP preparation, but such approaches would lead to inactivation of ASNase and thus could not be used.
The size, polydispersity index (PDI < 5 and unimodal size distribution), and entrapment efficiency of nanoparticles
CS (% w/ v)/TPP (% w/ v)
138 ± 7
180 ± 8
224 ± 10
187 ± 9
209 ± 11
247 ± 10
Optimization of protein loading
The characteristics of ASNase II-loaded CSNPs prepared by CS/TPP 0.4%/0.095% ( w / v ) and loaded with different amounts of lyophilized ASNase II
Lyophilized protein (mg)
Zeta potential (mV)
Protein content (mg)
250 ± 11
+35.5 ± 2
0.701 ± 0.011
262 ± 10
+30.7 ± 2
1.464 ± 0.05
295 ± 9
+24.1 ± 3
2.244 ± 0.105
340 ± 12
+21.2 ± 3
3.048 ± 0.07
Entrapment efficiency, yield, and loading capacity of the nanoparticles were increased through an increase in the amount of applied protein. These results are in agreement with those of Yoshida et al.  who studied the adsorption of BSA onto ionically cross-linked CS. According to these results, the negatively charged peptide and protein molecules are supposed to be encapsulated more efficiently in a cationic CS polymer. At the pH 5.7, the negatively charged ASNase II molecules (pI ~ 4.9) with their spherical structure could compete with TPP ions to electrostatically react with CS. In other words, ASNase II not only did not interfere with the formation of CSNPs but also might have helped to form CSNPs. The zeta potentials of ASNase II-loaded CSNPs were decreased from +35.5 ± 2 to +21.2 ± 3 mV when the protein contents of CSNPs were increased. Decline in the zeta potential could be explained by the reduction in - NH3+ groups on the CS because of further protein loading. In addition to TPP, the negative groups on the surface of ASNase II were counteracted with the positively charged - NH3+ groups of CS during the cross-linking process. Moreover, TPP could counteract with the positively charged - NH3+ groups on the surface of ASNase II and compact the enzyme both inside and on the surface of the particle. Particles possessing a zeta potential of about 20 to 25 mV may sometimes be considered relatively stable . However, having a sufficient zeta potential is extremely important for the role of nanoparticles as carriers for drugs or proteins; the nanoparticles must be capable of ionically holding active molecules or biomolecules. Nanoparticle used for the final characterization were loaded with 4 mg lyophilized ASNase II.
Fourier transform infrared spectrometry analysis
Morphology studies for the nanoparticles
In vitro ASNase II release
CS forms colloidal particles and entraps bioactive molecules both inside and on the surface of such particles. The mechanisms that have been reported to be involved include chemical cross-linking, ionic cross-linking, and ionic complexation . CS degrades with time in the presence of enzymes (i.e., lysozyme) when inserted into biological environments . However, it has also been found that CSNPs synthesized by ionotropic gelation lose their integrity in aqueous media even in the absence of enzymes. Most drug release profiles from CSNPs exhibit an initial burst release, presumably from the particle surface, followed by a sustained release driven by diffusion of drug through the polymer wall and polymer erosion [10, 42]. Gan and Wang  investigated the in vitro release of BSA from CSNPs. They concluded that the burst is more likely a consequence of rapid surface desorption of large amounts of protein molecules from a huge specific surface area provided by large numbers of particles at nanoscale, and a larger proportion of protein molecules may not be truly embedded in the nanoparticles' inner structure.
Effect of pH on free and immobilized enzyme activity and stability
The thermostability of the free and immobilized ASNase II
In vitro half-life of the immobilized and free ASNase II
The ionotropic gelation method used to prepare ASNase II-loaded CSNPs was so milder than those reported for PLGA , hydrogel-magnetic  and liposome  nanoparticle preparation. Wolf et al.  reported that during the ASNase II-PLGA nanosphere preparation, contact with lipophilic interfaces provokes protein denaturation and also necessary shear forces and cavitation stress for the formation of nanodroplets inactivate the enzyme. Gaspar et al.  reported that the use of the liposome-encapsulated ASNase II improved the survival of animals with asparagine-dependent P1534 tumors compared with free enzyme. One of the drawbacks of the use of liposomes is the fast elimination from the blood and capture of the liposomal preparations by the cells of the reticulo-endothelial system, primarily in the liver. A number of developments have aimed to reduce this problem, including coating the liposome surface with inert, biocompatible polymers, such as polyethylene glycol (PEG), to slow down the clearance of liposomes . Although PEG remains the gold standard for the steric protection of liposomes , it creates an impermeable layer over the liposome surface  which could decrease availability of blood asparagines to encapsulated ASNase II. However, research in nanomedicine offers a unique platform for a variety of manipulations that can further enhance the value of the delivered drugs.
It could be assumed by this study that, when the CSNPs are loaded with hydrophilic macromolecules or drugs, the interactions between them and the gel network can effectively make particles much more stable. The preparation of ASNase II-loaded CSNPs was based on an ionotropic interaction between the positively charged CS and the negatively charged ASNase II and TPP. The negatively charged ASNase II was able to link CS chains electrostatically at pH ~ 5.7 before the addition of the polyanion. Such ASNase II behavior was previously observed in DEAE- Sepharose column by positively charged amine groups of DEAE. ASNase II-CS interactions would be strengthened by adding a polyanion and rising pH. So, it could be assumed that CS networks were formed through two cross-linkers of TPP and ASNase II, and the drug itself helped particle formation that is of great interest in pharmaceutical productions. The pH and thermal stability, release, and half-life of ASNase II were evaluated. Compared to the free ASNase II, the immobilized enzyme was more resistant to alkaline pH (8.5 to 9.5) and to high temperatures. ASNase II release could be influenced by pH and the ionic strength of the medium. The immobilized enzyme had an increased half activity time of about 23 days in the low ionic strength solution and about 6.4 days in the high ionic strength solution. This in vitro study would provide an impetus for the future in vivo investigations. Further studies will be needed to find a suitable particle size and charge, biological responses, and administration route to apply in drug delivery and in vivo use.
We would like to thank the members of the Biotechnology Department of Razi Vaccine and Serum Research Institute for their help. This work was supported partly by Iran Nanotechnology Initiative Council and Hamadan University of Medical Sciences.
- Narta UK, Kanwar SS, Azmi W: Pharmacological and clinical evaluation of L-asparaginase in the treatment of leukemia. Crit Rev Oncol Hematol 2007, 61: 208–221. 10.1016/j.critrevonc.2006.07.009View ArticleGoogle Scholar
- Pasut G, Sergi M, Veronese FM: Anti-cancer PEG-enzymes: 30 years old, but still a current approach. Adv Drug Deliv Rev 2008, 60: 69–78. 10.1016/j.addr.2007.04.018View ArticleGoogle Scholar
- Wolf M, Wirth M, Pittner F, Gabor F: Stabilisation and determination of the biological activity of L-asparaginase in poly(D, L-lactide-co-glycolide) nanospheres. Int J Pharm 2003, 256: 141–152. 10.1016/S0378-5173(03)00071-1View ArticleGoogle Scholar
- Matsushima A, Nishimura H, Ashihara Y, Yokota Y, Inada Y: Modification of E. coli asparaginase with 2,4-bis(O-methoxypolyethylene glycol)-6-chloro-S-triazine(activated PEG2); disappearance of binding ability towards anti-serum and retention of enzymic activity. Chem Lett 1980, 103: 773–776.View ArticleGoogle Scholar
- Uren JR, Hargis BJ, Beardsley P: Immunological and pharmacological characterization of poly-DL-alanyl-modified Erwinia carotovora L-asparaginase. Cancer Res 1982, 42: 4068–4071.Google Scholar
- Wileman T, Foster RL, Elliot PNC: Soluble asparaginase-dextran conjugates show increased circulatory persistence and lowered antigen reactivity. J Pharm Pharmacol 1986, 38: 264–271. 10.1111/j.2042-7158.1986.tb04564.xView ArticleGoogle Scholar
- Gaspar MM, Perez-Soler R, Cruz ME: Biological characterization of L-asparaginase liposomal formulations. Cancer Chemother Pharmacol 1996, 38: 373–377. 10.1007/s002800050497View ArticleGoogle Scholar
- Gasper MM, Blanco D, Cruz ME, Alonso MJ: Formulation of L-asparaginase-loaded poly(lactide-co-glycolide) nanocapsules: influence of polymer properties on enzyme loading, activity and in vitro release. J Control Release 1998, 52: 53–62. 10.1016/S0168-3659(97)00196-XView ArticleGoogle Scholar
- Teodor E, Litescu SC, Lazar V, Somoghi R: Hydrogel-magnetic nanoparticles with immobilized L-asparaginase for biomedical applications. J Mater Sci Mater Med 2009, 20: 1307–1314. 10.1007/s10856-008-3684-yView ArticleGoogle Scholar
- Bhattarai N, Ramay HR, Chou SH, Zhang M: Chitosan and lactic acid-grafted chitosan nanoparticles as carriers for prolonged drug delivery. Int J Nanomedicine 2006, 1: 181–187. 10.2147/nano.2006.1.2.181View ArticleGoogle Scholar
- Bernkop-Schnürch A: Chitosan and its derivatives: potential excipients for peroral peptide delivery systems. Int J Pharm 2000, 194: 1–13. 10.1016/S0378-5173(99)00365-8View ArticleGoogle Scholar
- Guang Liu W, De Yao K: Chitosan and its derivatives—a promising non-viral vector for gene transfection. J Control Release 2002, 83: 1–11. 10.1016/S0168-3659(02)00144-XView ArticleGoogle Scholar
- Bodmeier R, Chen HG, Paeratakul O: A novel approach to the oral delivery of micro and nanoparticles. Pharm Res 1989, 6: 413–417. 10.1023/A:1015987516796View ArticleGoogle Scholar
- Calvo P, Remuñán-López C, Vila-Jato JL, Alonso MJ: Novel hydrophilic chitosan-polyethylene oxide nanoparticles as protein carriers. J Appl Polym Sci 1997, 63: 125–132. 10.1002/(SICI)1097-4628(19970103)63:1<125::AID-APP13>3.0.CO;2-4View ArticleGoogle Scholar
- Sun P, Li P, Li YM, Wei Q, Tian LH: A pH-sensitive chitosan-tripolyphosphate hydrogel beads for controlled glipizide delivery. J Biomed Mater Res B Appl Biomater 2011, 97: 175–183.View ArticleGoogle Scholar
- Wang JJ, Zeng ZW, Xiao RZ, Xie T, Zhou GL, Zhan GL, Shu Ling Wang SL: Recent advances of chitosan nanoparticles as drug carriers. Int J Nanomedicine 2011, 6: 765–774.Google Scholar
- Wang N, Gunn J, Zhang M: Chitosan-based hydrogels for controlled, localized drug delivery. Adv Drug Deliv Rev 2010, 62: 83–99. 10.1016/j.addr.2009.07.019View ArticleGoogle Scholar
- Zhang HL, Wu SH, Tao Y, Zang LQ, Su ZQ: Preparation and characterization of water-soluble chitosan nanoparticles as protein delivery system. J Nano Mat 2010, 2010: 1–5.Google Scholar
- Bahreini E, Aghaiypour K, Abbasalipourkabir R, Goodarzi MT, Saidijam M, Safavieh SS: An optimized protocol for over-production of recombinant protein expression in Escherichia coli . Prep Biochem Biotechnol 2014, 44: 510–528. 10.1080/10826068.2013.833116View ArticleGoogle Scholar
- Imada A, Igarasi S, Nakahama K, Isono M: Asparaginase and glutaminase activities of micro-organisms. J Gen Microbiol 1973, 76: 85–99. 10.1099/00221287-76-1-85View ArticleGoogle Scholar
- Lowry OH, Rosebrough NJ, Farr AL, Randall RJ: Protein measurement with the folin phenol regent. J Biol Chem 1951, 193: 265–275.Google Scholar
- Kawashima Y, Handa T, Kasai A, Takenaka H, Lin SY, Ando Y: Novel method for the preparation of controlled-release theophylline granules coated with a polyelectrolyte complex of sodium polyphosphate-chitosan. J Pharm Sci 1985, 74: 264–268. 10.1002/jps.2600740308View ArticleGoogle Scholar
- Harms E, Wehner A, Aung HP, Röhm KH: A catalytic role for threonine-12 of E. coli asparaginase II as established by site-directed mutagenesis. FEBS Lett 1991, 285: 55–58. 10.1016/0014-5793(91)80723-GView ArticleGoogle Scholar
- Bajaj G, Van Alstine WG, Yeo Y: Zwitterionic chitosan derivative, a new biocompatible pharmaceutical excipient, prevents endotoxin-mediated cytokine release. PLoS One 2012, 7: e30899. 10.1371/journal.pone.0030899View ArticleGoogle Scholar
- Mao HQ, Roy K, Troung-Le VL, Janes KA, Lin KY, Wang Y, August JT, Leong KW: Chitosan-DNA nanoparticles as gene carriers: synthesis, characterization and transfection efficiency. J Control Release 2001, 70: 399–421. 10.1016/S0168-3659(00)00361-8View ArticleGoogle Scholar
- Greenquist AC, Wriston JC Jr: Chemical evidence for identical subunits in L-asparaginase from Escherichia coli B. Arch Biochem Biophys 1972, 152: 280–286. 10.1016/0003-9861(72)90216-0View ArticleGoogle Scholar
- Swain AL, Jaskólski M, Housset D, Rao JK, Wlodawer A: Crystal structure of Escherichia coli L-asparaginase, an enzyme used in cancer therapy. Proc Natl Acad Sci U S A 1993, 90: 1474–1478. 10.1073/pnas.90.4.1474View ArticleGoogle Scholar
- Huang Y, Lapitsky Y: Monovalent salt enhances colloidal stability during the formation of chitosan/tripolyphosphate microgels. Langmuir 2011, 27: 10392–10399. 10.1021/la201194aView ArticleGoogle Scholar
- Gan Q, Wang T: Chitosan nanoparticles as protein delivery carrier—systematic examination of fabrication conditions for efficient loading and release. Colloids Surf B: Biointerfaces 2007, 59: 24–34. 10.1016/j.colsurfb.2007.04.009View ArticleGoogle Scholar
- Lavertu M, Méthot S, Tran-Khanh N, Buschmann MD: High efficiency gene transfer using chitosan/DNA nanoparticles with specific combinations of molecular weight and degree of deacetylation. Biomaterials 2006, 27: 4815–4824. 10.1016/j.biomaterials.2006.04.029View ArticleGoogle Scholar
- López-León T, Carvalho EL, Seijo B, Ortega-Vinuesa JL, Bastos-González D, Ortega-Vinuesa JL, Bastos-González D: Physicochemical characterization of chitosan nanoparticles: electrokinetic and stability behavior. J Colloid Interface Sci 2005, 283: 344–351. 10.1016/j.jcis.2004.08.186View ArticleGoogle Scholar
- Alsarra IA, Neau SH, Howard MA: Effects of preparative parameters on the properties of chitosan hydrogel beads containing Candida rugosa lipase. Biomaterials 2004, 25: 2645–2655. 10.1016/j.biomaterials.2003.09.051View ArticleGoogle Scholar
- Wang R, Xia B, Li BJ, Peng SL, Ding LS, Zhang S: Semi-permeable nanocapsules of konjac glucomannan–chitosan for enzyme immobilization. Int J Pharm 2008, 364: 102–107. 10.1016/j.ijpharm.2008.07.026View ArticleGoogle Scholar
- De Jong WH, Borm PJ: Drug delivery and nanoparticles: applications and hazards. Int J Nanomedicine 2008, 3: 133–149.View ArticleGoogle Scholar
- Nagpal K, Singh SK, Mishra DN: Chitosan nanoparticles: a promising system in novel drug delivery. Chem Pharm Bull (Tokyo) 2010, 58: 1423–1430. 10.1248/cpb.58.1423View ArticleGoogle Scholar
- Yoshida H, Nishihara H, Kataoka T: Adsorption of BSA on strongly basic chitosan: equilibria. Biotechnol Bioeng 1994, 43: 1087–1093. 10.1002/bit.260431112View ArticleGoogle Scholar
- Lee DW, Powers K, Baney R: Physicochemical properties and blood compatibility of acylated chitosan nanoparticles. Carbohyd Polym 2004, 58: 371–377. 10.1016/j.carbpol.2004.06.033View ArticleGoogle Scholar
- Wu Y, Yang W, Wang C, Hu J, Fu S: Chitosan nanoparticles as a novel delivery system for ammonium glycyrrhizinate. Int J Pharm 2005, 295: 235–245. 10.1016/j.ijpharm.2005.01.042View ArticleGoogle Scholar
- Knaul JZ, Hudson SM, Creber KAM: Improved mechanical properties of chitosan fibers. J Appl Polym Sci 1999, 72: 1721–1732. 10.1002/(SICI)1097-4628(19990624)72:13<1721::AID-APP8>3.0.CO;2-VView ArticleGoogle Scholar
- Xu Y, Du Y: Effect of molecular structure of chitosan on protein delivery properties of chitosan nanoparticles. Int J Pharm 2003, 250: 215–226. 10.1016/S0378-5173(02)00548-3View ArticleGoogle Scholar
- Yang YM, Hu W, Wang XD, Gu XS: The controlling biodegradation of chitosan fibers by N-acetylation in vitro and in vivo. J Mater Sci Mater Med 2007, 18: 2117–2121. 10.1007/s10856-007-3013-xView ArticleGoogle Scholar
- Amidi M, Mastrobattista E, Jiskoot W, Hennink WE: Chitosan-based delivery systems for protein therapeutics and antigens. Adv Drug Deliv Rev 2010, 62: 59–82. 10.1016/j.addr.2009.11.009View ArticleGoogle Scholar
- Wang AZ, Gu F, Zhang L, Chan JM, Radovic-Moreno A, Shaikh MR, Farokhzad OC: Biofunctionalized targeted nanoparticles for therapeutic applications. Expert Opin Biol Ther 2008, 8: 1063–1070. 10.1517/147125184.108.40.2063View ArticleGoogle Scholar
- Leroux L, Hatim Z, Frèche M, Lacout JL: Effects of various adjuvants (lactic acid, glycerol, and chitosan) on the injectability of a calcium phosphate cement. Bone 1999, 25: 31–34. 10.1016/S8756-3282(99)00130-1View ArticleGoogle Scholar
- Singh A, Narvi SS, Dutta PK, Pandey ND: External stimuli response on a novel chitosan hydrogel crosslinked with formaldehyde. Bull Mater Sci 2006, 29: 233–238. 10.1007/BF02706490View ArticleGoogle Scholar
- Giannotti MI, Esteban O, Oliva M, García-Parajo MAF, Sanz F: pH-responsive polysaccharide-based polyelectrolyte complexes as nanocarriers for lysosomal delivery of therapeutic proteins. Biomacromolecules 2011, 12: 2524–2533. 10.1021/bm2003384View ArticleGoogle Scholar
- Shu XZ, Zhu KJ: A novel approach to prepare tripolyphosphate/chitosan complex beads for controlled release drug delivery. Int J Pharm 2000, 201: 51–58. 10.1016/S0378-5173(00)00403-8View ArticleGoogle Scholar
- Massart R: Preparation of aqueous magnetic liquids in alkaline and acidic media. IEEE Trans Magn 1981, 17: 1247–1248. 10.1109/TMAG.1981.1061188View ArticleGoogle Scholar
- Klibanov AL, Maruyama K, Torchilin VP, Huang L: Amphipatic polyethyleneglycols effectively prolong the circulation time of liposomes. FEBS Lett 1990, 268: 235–238. 10.1016/0014-5793(90)81016-HView ArticleGoogle Scholar
- Torchilin VP: Recent advances with liposomes as pharmaceutical carriers. Nat Rev Drug Discovery 2005, 4: 145–160. 10.1038/nrd1632View ArticleGoogle Scholar
- Torchilin VP, Omelyanenko VG, Papisov MI, Bogdanov AA Jr, Trubetskoy VS, Herron JN, Gentry CA: Poly(ethylene glycol) on the liposome surface: on the mechanism of polymer-coated liposome longevity. Biochim Biophys Acta 1994, 1195: 11–20. 10.1016/0005-2736(94)90003-5View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.